**__________________________________________________________________________________________**

*Citation for published version:*

Okereke, Michael I (2016) Flexural response of polypropylene/E-glass fibre reinforced unidirectional composites. Composites Part B: Engineering. ISSN 1359-8368

(doi:10.1016/j.compositesb.2016.01.007)

*Publisher’s version available at:*

http://dx.doi.org/10.1016/j.compositesb.2016.01.007

**__________________________________________________________________________________________**

**Please note that where the full text version provided on GALA is not the final published **
**version, the version made available will be the most up-to-date full-text (post-print) version as **
**provided by the author(s). Where possible, or if citing, it is recommended that the publisher’s **
**(definitive) version be consulted to ensure any subsequent changes to the text are noted.**

*Citation for this version held on GALA:*

Okereke, Michael I (2016) Flexural response of polypropylene/E-glass fibre reinforced unidirectional composites. London: Greenwich Academic Literature Archive.

Available at: http://gala.gre.ac.uk/14330/

**__________________________________________________________________________________________**
**Contact: gala@gre.ac.uk**

Flexural response of polypropylene/E-glass fibre reinforced unidirectional composites Michael I. Okereke

PII: S1359-8368(16)00008-1

DOI: 10.1016/j.compositesb.2016.01.007 Reference: JCOMB 3962

To appear in: *Composites Part B*
Received Date: 23 November 2015
Revised Date: 5 January 2016
Accepted Date: 7 January 2016

Please cite this article as: Okereke MI, Flexural response of polypropylene/E-glass fibre reinforced
*unidirectional composites, Composites Part B (2016), doi: 10.1016/j.compositesb.2016.01.007.*
This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to
our customers we are providing this early version of the manuscript. The manuscript will undergo
copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please
note that during the production process errors may be discovered which could affect the content, and all
legal disclaimers that apply to the journal pertain.

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

→→→ REVISED VERSION OF MANUSCRIPT JCOMB-S-15-02629 ←←←

### Flexural response of polypropylene/E-glass fibre reinforced

### unidirectional composites.

Michael I. Okereke∗

*Department of Engineering Science, University of Greenwich, Kent, United Kingdom*

Abstract

This paper presents a study of the flexural response of continuous E-glass fibre reinforced
polypropylene composites. Experiments were designed to investigate monotonic and cyclic
flexural response using three point bending test for laminates with different angle-ply and
cross-ply arrangements. Results show that the monotonic and cyclic flexural response of the
composites are influenced by the plastic deformation of the matrix. The study observed that
increasing numbers of cyclic loads led to significant energy dissipation, stiffness reduction
and micro-damage accumulation within the composite and especially at the matrix-fibre
interface. Significant energy dissipation and damage were observed to dominate the first
load-unload cycle. With subsequent cycles, the magnitude of energy dissipation and global
damage reduces to a threshold value which is cycle independent. This study has also
devel-oped a phenomenological model to predict the dependence of energy dissipation with number
of cycles. The experimental data generated here will be useful in the development of holistic
macroscale constitutive models and finite element studies of the chosen test composite.
*Keywords: A. Polymer Matrix Composites, A. Plytron*TM, B. Three Point Bending, B.
Cyclic Flexural Response

1. Introduction 1

In automotive and aerospace industries, the use of thermoplastics as matrix systems of 2

fibre reinforced composites has continued to grow steadily. This is largely due to the ma-3

terials’ recyclability and ability to be processed rapidly. Higher strength-to-weight ratios, 4

better chemical and impact resistance, improved fracture toughness over thermosets and 5

enhanced fatigue strength are some other reasons why thermoplastic composites are becom-6

ing the material of choice for replacing traditional materials as steel, aluminum, wood, etc 7

∗_{Corresponding Address:}_{Department of Engineering Science, University of Greenwich, Medway }

Cam-pus, Kent, ME4 4TB, United Kingdom Phone: +44 (0) 1634 88 3580 Fax: +44 (0) 1634 88 3153.

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

[1–4]. One particularly promising type of thermoplastic composites is cost-effective, con-8

tinuous E-glass fibre reinforced polypropylene-matrix composites. These have potential as 9

thermoformable automotive body parts [5, 6], and have attracted attention for example as 10

possible components of composite integral body armours [7, 8], and of fibre-metal laminate 11

sandwich structures designed for ballistic protection [9–11]. 12

Although the use of thermoplastic composites is growing steadily, its application in struc-13

tural components is inhibited by limited set of reliable experimental data about their me-14

chanical response, especially the cyclic flexural response [12,13]. Bending collapse of vehicles 15

is a dominant failure mode experienced during oblique or side collisions of vehicles hence 16

the interest in them in this paper [14]. In order to encourage the widespread adoption 17

of thermoplastic matrix composites in different engineering applications, it is essential to 18

widen the current understanding of their mechanical response. This demands research on 19

both experimental investigations and numerical modelling of these composites. This work 20

aims to generate experimental data on monotonic and cyclic flexural response of a contin-21

uous E-glass fibre reinforced polypropylene matrix composites marketed by the trade name 22

PlytronTM [15, 16]. The interest in PlytronTM stems from the fact that it is widely used in 23

automotive parts and has an unusually high volume fraction of matrix (i.e. 65%) compared 24

with other thermoplastic composites. 25

A few authors have carried out experiments on polypropylene-based composites and such 26

studies were focussed on the effect of processing histories on the mechanical performance 27

of the test materials. Al-Zubaidy and co-workers [17] investigated the tensile and shear 28

properties of orthotropic glass-polypropylene composites made under different processing 29

conditions and found that crossply laminates had excellent tensile and shear properties 30

with interlaminar shear strength (ILSS) being 2.5 times the ILSS of other thermoplastics 31

composites made using the same processing history. Al-Zubaidys work also showed that 32

PlytronTM had comparatively higher fracture toughness compared to similar composites and 33

this was attributed to the high coupling between the fibre and the matrix components. 34

Data obtained from impact studies of commingled E-glass fibre polypropylene compo-35

sites by Santulli and co-workers [18] were compared with those of PlytronTM and the authors 36

reported better mechanical properties of PlytronTM than similar polypropylene-based com-37

posites. In particular, the flexural response of PlytronTMwas comparable to the properties of 38

the more aligned 4:1 weave TwintexTM composite. This observation was attributed to both 39

the non-crimped form of the fibre reinforcement as well as improved impregnation achieved in 40

PlytronTM composites. These excellent properties of make PlytronTM an interesting material 41

to study. 42

As well as Al-Zubaidy’s [17] and Santulli’s [18] works, another study by Rijsdijk and 43

co-workers [19] assessed the role of interphase modification on the mechanical response of 44

polypropylene-based composites. The work concluded that any modifications affected sig-45

nificantly those composite properties that depend on the interphase, like transverse, shear 46

and compressive strength. Thomason and colleagues [20,21] confirmed this by carrying out 47

a single-fibre pullout test on composites modified using different interface coatings. The 48

flexural strength of the glass fibre/polypropylene composite was found to vary by a factor 49

of two depending on the type of glass fibre coating used. 50

Most recently, Hagstrand and co-workers [22] investigated the effect of percentage void 51

volume fraction to the mechanical behaviour of commingled E-glass fibre polypropylene-52

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

matrix composites. They hoped that by optimizing manufacturing techniques to minimize 53

formation of voids, composites of improved mechanical responses could be obtained. The 54

authors found the presence of voids had negative effects on the flexural modulus and strength 55

except surprisingly the flexural rigidity, EI which was found to increase by 2% with each 1% 56

increase in percentage void volume fraction. It was thought that the presence of voids led 57

to increase in dimensions of tested specimen hence increasing the moment of inertia. 58

Simeoli and colleagues [23] reported that changes to the interface strength of PP/E-glass 59

fibre laminates affected their low velocity impact behaviour. By incorporating a compatibi-60

lizer, the authors found that the flexural modulus and the strength of the composite were 61

significantly increased. The authors observed that interface failure occurred at low strains 62

for non-compatibilizer-strengthened composites. The authors explained that the failure re-63

sulted from large energy dissipation occurring at the polymer/fibre matrix. This conclusion 64

was confirmed using what they described as locked-in thermographic analysis of the tested 65

specimen [24]. 66

This short review into mechanical (especially flexural) response of PP/E-glass fibre com-67

posites highlights the sustained research interest in such composites but most significantly 68

shows the importance of accumulating more experimental data on thermoplastic composites 69

with dominant matrix composition as PlytronTM . The development of micromechanical and 70

macroscale constitutive models of thermoplastic composites will benefit immensely from re-71

liable experimental data generated through uniaxial, flexural, shear and fatigue testing of 72

such composites. Motivated by this need, this paper presents experimental data on a series 73

of experiments carried out with specific focus of understanding the monotonic and short 74

cycle flexural behaviour of continuous E-glass fibre polypropylene matrix composite. 75

2. Test material 76

*2.1. Plytron*TM *: a continuous polypropylene/E-glass fibre composite*
77

The test material under investigation is continuous polypropylene/E-glass fibre reinforced 78

composite. PlytronTM is the registered trademark for this continuous unidirectional glass 79

fibre reinforced polypropylene composite made by a Swiss company called Gurit Suprem 80

but now trades as Gurit. It is a 100% consolidated, thermoplastic composite which is 81

commercially available as prepreg tapes of 300 mm wide, 0.25 - 0.28 mm thick and roll 82

length of 400 m. The reinforcement is obtained with continuous unidirectional glass fibres 83

with a weight ratio of 60-wt% (or 35-vol% fibre)[15, 16]. The matrix phase is a blend of 84

standard polypropylene and 5% master-batch compound. The master-batch contains carbon 85

black among other proprietary ingredients, hence giving the composite a black appearance. 86

Plytron is commonly used in the automobile industries. Table 1 gives the manufacturer’s 87

data for typical mechanical properties of PlytronTM based on experiments performed on 88

unidirectional and symmetric cross-ply laminates.1

89

*2.2. Manufacture of test material*
90

Composite laminates were prepared from PlytronTM prepreg tapes through compression 91

moulding in a heated press. In preparing test specimens, plies of dimensions of 140 × 140 92

1

*The n in [0*n] and [(0/90)n]s within Table 1 represents the number of plies and takes values ranging

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

Table 1: Physical and Mechanical Properties of PlytronTM [15,16].

Properties Units [0n] [(0/90)n]s

Density, ρ g/cm3

1.48 1.48

Fibre Content gew% 60

vol% 35

Tensile Strength, Xt MPa 680 360

Tensile Modulus, Exx GPa 22.5 16

Elongation at break, ǫf % 2.1 2.5

Flexural Strength, σb,max MPa 570 350

Flexural Modulus, Eb GPa 22 16.5

Thermal Expansion Coefficient,αT µm/mK 7 20

mm were cut from the reel of prepreg tapes. The plies were then arranged according to 93

a desired stacking sequence and placed inside a picture-frame mould specially designed for 94

the moulding of test specimens. A PTFE spray was applied onto the inside lid and inside 95

base plates of the mould to help in easy removal of the laminates after moulding. Each 96

moulding was made under the optimal processing conditions of: (a) temperature of heated 97

press platens: 22o_{− 250}o _{C, (b) pressure applied on top and bottom of the mould: 1.5 - 2.0}
98

MPa, (c) number of plies per laminate: 12 plies (for a laminate of thickness 3.0mm), and 99

(d) processing cycle: 25 mins (comprising 10 mins heating up, 5 minutes dwell time and 100

10 mins cooling period). Typical heating and cooling rates were 15o _{C/min and 20}o _{C/min}
101

respectively. Successive loading and unloading cycles, over 30-second intervals from start of 102

heating, were applied to ensure that any trapped air pockets that would cause voiding were 103

forced out. The mould was cooled from the set platen temperature to room temperature by 104

water cooling of the heated platens. 105

*2.3. Microscopy of test composite*
106

The microstructure of the manufactured test material was assessed using optical and 107

scanning electron microscopy studies. These studies were carried out to explore the nature 108

of the interaction/bonding between the matrix and the glass fibre reinforcement and also 109

check for the absence of voids in order to ensure the suitability of the test specimens for 110

flexural tests. The laminates under investigation have a unidirectional layup. They were 111

cut into specimens of dimensions of 10 × 10 mm2

using a band-saw with fine blades. The 112

specimens were mounted on Bakelite and polished for between 40-60 mins using Kemet

113

self-adhesive cloths diamond compound of grade 6-KD-C2 and a lubricating fluid. Once 114

satisfactory polishing was achieved, the test specimens were imaged in an Alicona Infinite 115

Focus profilometer set in 2D imaging mode. Micrographs were obtained in the through-116

thickness section of the test materials. This assessment reveals that the microstructure of 117

PlytronTM *consists of clearly defined regions of matrix-rich and fibre-rich zones (see Figures*
118

*1(a)* *to* *1(c)*) - typical of laminated composites. Scanning electron microscopy was used

119

to obtain micrographs demonstrating excellent bonding between the matrix and fibre as 120

*shown in Figure* *1(d)*. This confirms that the laminate making process achieved high level
121

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

of consolidation. In all the assessed micrographs, voiding was very minimal. 122

(a) (b)

(c) (d)

Figure 1: Optical micrographs of a typical test specimen showing: (a) banded arrangement of fibre (grey circles) within the matrix (black region);(b)random arrangement of fibres within fibre-rich zone (A); and

(c)limited distribution of fibres within matrix-rich zone (B); as well as(d)zoomed-in view of two individual fibres: showing good fibre-matrix consolidation, and absence of voids.

3. Experimental test setup and specimen design 123

Compression moulded laminates with different fibre orientations were cut into beam spec-124

imens and tested by three-point bending test. Symmetric laminates of stacking sequences 125

were studied where θ = 0o_{, 15}o_{, 30}o_{, 45}o_{, 60}o_{, 75}o_{, and 90}o _{and n = 5. Also, cross-ply }
speci-126

mens of stacking sequence [(0/90)5]s *were also tested. Figure* *2* shows the geometry of three
127

point bending test specimens. 128

According to theISO 14125:1998 test standard for flexural test of fibre-reinforced plastic

129

composites, the dimension of the test specimen was chosen as 70 × 20 × 2.8 mm3

. All tests 130

were carried out using an Instron Series IX Automated Materials Testing System 4204. A 131

*three-point bending test rig, shown in Figure* *3*, was fitted to the Instron machine such
132

that when tensile load is applied on the end supports of the test specimen, the specimen 133

responds in bending around a mid-span fulcrum support of radius 2.5 mm. Flexural forces 134

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

b = 20mm Length, l = 90mm t = 2.5 mmFigure 2: Design of a three-point bending test specimen.

were measured using a 5 kN load cell while the deflection of the beam was measured by 135

crosshead displacement. Tests were carried at crosshead speed of 5 mm/min.
136
Original
specimen
**P**
Span, S
**0.5 P** **0.5 P**
**R = 2.5 mm**
Deformed
specimen

Figure 3: Schematic representation of a three-point bending test rig highlighting the test specimen and loading arrangement that enforces the bending response of the test material.

4. Test Results 137

*4.1. Monotonic flexural tests*
138

The flexural response of PlytronTM is presented in plots of Force, F [N] against mid-span 139

deflection of the beam, δ [mm]. The maximum flexural force, Fmax is identified as the peak 140

*force on the flexural force-deflection plot. Figures4(a)-4(h)*show plots of flexural responses
141

of PlytronTM laminates for fibre orientations from 0o _{to 90}o_{. The 0}o _{test specimens refer to}
142

unidirectional composites where the fibre-axis aligns with the longitudinal neutral axis of 143

the test specimen. The plot for the 0o _{laminates was dominated by the linear elasticity of}
144

*the fibre, as shown in Figure* *4(a)*. Similarly, the flexural response of 90o _{test specimens was}
145

determined transverse to the fibre’s longitudinal direction. In this later case, the flexural 146

*response was dominated by the nonlinear viscoelasticity of the matrix, as shown in Figure*
147

*4(f )*. Also, three-point bending tests were carried out on cross-ply laminates and the result
148

*is shown in Figure* *4(g)*. The comparison showing the full range of the monotonic flexural
149

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

*response of this class of composite is shown in Figure* *4(h)* which shows the dependence of
150

the composite flexural response with fibre orientations. These results show, as expected that 151

the flexural response of the thermoplastic matrix composite was linear elastic till yield for 152

fibre-dominated directions (i.e. for fibre orientation, θ = 00 , 150

and [(0/90)5]_{s}) while for the
153

other fibre orientations, the plasticity of the matrix dominated the flexural response. 154

(a) (b) (c)

(d) (e) (f)

(g) (h)

Figure 4: Monotonic flexural response of PlytronTM laminates for the following stacking sequences: (a)[010],

(b)[(±15)5]s,(c)[(±45)5]s,(d)[(±60)5]s,(e)[(±75)5]s,(f)[9010],(g)[(0/90)5]s,(h)comparison of all fibre

orientations.

*4.2. Short cycle flexural tests*
155

The aim here was to investigate the flexural response of PlytronTM under short cycle 156

loading. Similar specimen design and test rig used in the previous section were used in these 157

tests. The test specimens were tested in the Instron Machine in displacement-control mode. 158

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

A limiting deflection, δlimit *(herein referred to as cyclic deflection limit (CDL)), was chosen*
159

such that deflection does not exceed 80% of the flexural peak load (i.e. δlimit ≤ 80%) for 160

each laminate under consideration. This δlimit also ensures that the loading regime exceeds 161

the elastic limit of the laminates but not approach the unstable region of onset of failure. 162

*As a result, it was possible to investigate as reported in Section* *5.4*, the accumulation of
163

microscopic damage until eventual failure. 164

All test specimens were subject to cyclic loads of up to 5 cycles and typical force-deflection 165

*plots for a cross-ply and four angle-ply laminates are shown in Figure* *5(a)* *-* *5(e)*. Only 5
166

cycles were chosen as this study was aimed at short cycle fatigue. Traditionally, during 167

fatigue tests, tests specimens are subjected to hundreds of thousands of cycles, in order 168

to assess the cyclic response of the test material. For the purpose of this work, it has 169

*been observed, and reported later in Section* *5.3* that after the first three - five cycles, the
170

composite experiences a cycle independent energy dissipation which is the same irrespective 171

of increasing number of cycles. As a result, this work has focussed on the short cycle fatigue 172

of the test composite - in the region within which significant changes in the mechanical 173

response of the composite - is observed. 174 0 0.3 0.6 0.9 1.2 1.5 1.8 2.1 2.4 2.7 0 20 40 60 80 100 120 140 Deflection, [mm] F lex ura l F orc e, F [ N ] (a) 0 1 2 3 4 5 6 7 8 0 50 100 150 200 250 Deflection, [mm] F lex ura l F orc e, F [ N ] (b) 0 1 2 3 4 5 6 7 8 9 10 11 0 20 40 60 80 100 120 140 Deflection, [mm] F lex ura l F orc e, F [ N ] (c) 0 1 2 3 4 5 6 7 8 0 10 20 30 40 50 60 70 Deflection, [mm] F lex ura l F orc e, F [ N ] (d) 0 1 2 3 4 5 6 7 8 0 10 20 30 40 50 Deflection, [mm] F lex ura l F orc e, F [ N ] (e)

Figure 5: Short cycle flexural response of PlytronTM laminates for the following stacking sequences: (a)

cross-ply [(0/90)5]s; angle-plies: (b)[(±30)5]s,(c) [(±45)5]s,(d)[(±60)5]s, and(e)[(±75)5]slaminates.

5. Discussions 175

*5.1. The mechanics of the composite’s flexural response*
176

At very small deflections, δ ≪ t where t = thickness, the principles of classical lamina-177

tion theory [25, 26] can be applied to the analysis of the linear elastic flexural response of 178

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

the symmetric laminates tested here. Consider a simply supported rectangular plate of di-179

mensions: length, L, width, b and thickness, t subjected to bending. The moment-curvature 180

relationship [25] of a laminated composite plate is: 181 Mx(t) My(t) Mxy(t) = D11(t) D12(t) D16(t) D12(t) D22(t) D26(t) D16(t) D26(t) D66(t) κx(t) κy(t) κxy(t) . (1)

Here, Mx(t) is a rate-dependent bending moment per unit width of the beam about 182

the plane containing the bar axis; Dij(t) is rate-dependent laminate bending stiffness, for 183

i, j = 1, 2, 6 and κx(t) is the resulting rate-dependent curvature about the x-axis. For 184

ease of writing, the rate-dependence is assumed and not explicitly written, hence Mx(t) is 185

written as simply Mx, as well as flexural stress, σ(t) becomes σ. In a pure bending test, 186

κy = κxy *= 0. Therefore, the moment-curvature expression - based on Equation* *1* - for
187

analysing the three-point bending tests becomes: 188

Mx = κxD11 ⇒ M = bκ_{x}D11=
bD11

ρx

, (2)

where b = width of beam, M = total bending moment, and radius of curvature, ρx = κ−1x . 189

For a simply supported composite beam of span, L subjected to a three-point bending by a 190

concentrated force, F - imposed on the middle of the beam, the expression of the force per 191

unit deflection is: 192 F δ = 48EI L3 ⇒ EI = L3 48 F δ = D11. (3)

According to simple beam theory, Mx = κxEIx which implies that the expression for 193

the D11 *element of the bending stiffness matrix, D of the composite becomes equation* *3*.
194

The expressions for calculating the flexural strength, σmax and flexural modulus, Ef of the 195

PlytronTM *laminates are given in Equation* *4* . For calculating the strength and flexural
196

modulus of the test composite, the x-axis moment of inertia for a rectangular cross-section 197

beam is Ix = bt 3

12 and the following equation was used: 198

Strength : σmax = 3P L

2bt2, and Flexural Modulus : Ef =
1
4b
L
t
3
F
δ. (4)
*A MATLAB script called LamPower was created based on the principles of the *
com-199

monly used classical lamination theories[25] namely: rule of mixtures, Halpin-Tsai equations, 200

*Spencer’s square array model as well as simplified micromechanics equations of Chamis[27].*
201

Also, the much recently published closed-form micromechanics equations herein called Morais’ 202

*self-consistent model [*28] was also implemented within LamPower. The script was used to
203

generate the D-matrix for a given laminated stacking sequence, having specified the elastic 204

properties and volume fractions of the constituents as well as the ply size and the stacking 205

*sequence of the laminates. The output from LamPower was used to derive predicted flexural*
206

modulus used in the next section. 207

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

*5.2. Comparison of experiments with laminate theory predictions*
208

The objective here is to compare experimentally determined laminate bending stiffness 209

of PlytronTM *with predictions based on the classical laminate theory established in Section*
210

*5.1* above. In the expression for D11 *in Equation* *3*, the term F_{δ} (unit = [N/mm]) is the
211

*slope (for δ ≪ t) of the force-deflection plots of Figure* *4*. Using the deflection of δ = 0.5
212

*mm and the Modulus expression of Equation* *4, Figure* *4* data were used to determine the
213

laminate bending stiffness for all six fibre orientations. The properties of the fibre and 214

*matrix constituents, given in Table* *2*, were used to determine the D11 term of the
D-215

*matrix. Predicted values of the bending stiffness were determined using the LamPower*
216

implementation of the classical laminate theory. 217

Table 2: Typical room temperature properties of E-glass fibre reinforcement and isotropic semicrystalline polypropylene matrix used in PlytronTM .

Property Fibre Matrix Units

Density, ρ 2600 900 kg/m3

Young’s Modulus, E 73 1.308 GPa Tensile Strength, X 2250 40 MPa

Shear Modulus, G 31 0.46 GPa

In determining the predicted values, the size of each laminate ply was found to be 218

0.25 ± 0.002 mm. This was calculated from the plot of number of plies, N used per laminate 219

against thickness, t of the laminate. Six mouldings of different thicknesses ranging from 220

t = 2.5 mm to t = 10 mm were used. The ply size: 0.25 ± 0.002 mm, was determined 221

by substituting N = 1 (for one ply) into the linear function of plot of number of plies per 222

*laminate versus laminate thickness. Figure* *6*shows the comparison of the experimental and
223

predicted variation of the laminate flexural modulus, Ef with ply orientation, θ. The results 224

*in Figure* *6* show a good agreement, within experimental error, between the experimental
225

and predicted Ef *values for all fibre orientations based on the Morais self-consistent model*
226

[28]. According to this result, the Spencer’s square array model [25] and Chamis’ simplified 227

*micromechanics model [*27] established upper and lower bounds to the Ef values.
228

*5.3. Quantifying the energy dissipation for cyclic flexural response*
229

The stress-strain cyclic profile following a uniaxial fatigue test gives a measure of the 230

stiffness degradation or energy dissipation experienced by a test material. Similarly, the 231

force-deflection plot of a three-point bending tests as reported here can give information 232

of degradation of stiffness or energy dissipation as the uniaxial tests [29–31]. In order to 233

*quantify the cyclic flexural response, let us define an energy dissipation factor, ζ*d as in
234

*Equation* *5*:
235

Energy dissipation factor, ζd= 1 −

Eunloading Eloading

, (5)

where Eloading is the strain energy of the loading curve segment whilst Eunloading is the 236

strain energy of the unloading curve segment. These strain energies were determined as the 237

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

0 10 20 30 40 50 60 70 80 90 100 110 120 0 5 10 15 20 25 30Fibre Orientations, [deg]

F lex ura l M od ulu s , E f [ GP a]

Three-Point Bending Experiment Rules of Mixtures Model

Simplified Micromechanics Equations Spencer's Square Array Model Morais Self-consistent Model Halpin-Tsai Model with =1.20

Figure 6: Comparison of experimental and predicted flexural modulus, Ef. The prediction was based on

selected composite lamination theories. *Note: The error bars was determined by calculating the standard*
*deviation of the slope of the force-displacement plots for all the tested specimens per given fibre orientation*

areas under the appropriate curve segment. The areas were calculated numerically using the 238

trapezoidal rule. For the three-point bending test, the ζdparameter represents a quantitative 239

measure the energy dissipation following successive cyclic loading of the the material[29]. 240

Consider the cyclic flexural response of [(±45)5)]_{s} Plytron
TM

laminate, the test specimen 241

*was subjected to 5 cycles of flexural loading as shown in Figure* *7(a)* . The short cycle
242

flexural response the PlytronTM *laminates shown in Figure* *7(b)* indicates that at the end
243

of the unloading curve, the laminate does not return to zero deflection but there exists a 244

residual deflection. For the first cycle of the [(±45)5]s Plytron TM

laminate, the residual 245

deflection was 2.1 mm and by the fifth cycle, this has reduced 0.32 mm. Similarly, the area 246

under the load-unload curves evolves from 504 N-mm to 147 N-mm. 247

It is customary to represent ζd as a percentage, thus providing a measure of energy 248

*dissipation between successive cycles. Using the cyclic plots of Figure* *5* *and Equation* *5*,
249

the plots of energy dissipation factor, ζd against number of cycles, N for both angle-ply and 250

*cross-ply laminates are shown in Figure* *8. The plot of Figure* *8* shows that for increasing
251

angle, θ between the fibre and the main axis of bending, the percentage energy dissipation 252

factor, ζd increases. Cross-ply laminates show very small energy dissipation compared with 253

the angle-ply laminates. 254

*The data in Figure* *8* shows the most significant energy loss occurred between the first
255

two cycles. For example, for the [(±75)5]_{s} laminates, the percentage change in energy
256

dissipation ∆ζd = 70% − 46% = 24% whilst for the [(0/90)5]s laminates, ∆ζd = 3%. The 257

cyclic flexural response of the test composite indicates significant energy dissipation in those 258

laminate arrangements that experience significant plastic deformation. Therefore, structural 259

applications requiring significant energy absorption in the first loading cycle can be made 260

based on the test material with the [(±45)5]s] laminate arrangement. 261

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

0 2 4 6 8 10 12 14 0 25 50 75 100 125 150 Deflection, [mm] F le xu ra l F o rce , F [ N ] Cycle 1 Cycle 2 Cycle 3 Cycle 4 Cycle 5 (a) 0 2 4 6 8 10 0 25 50 75 100 125 150 Deflection, [mm] F le xu ra l F o rce , F [ N ] Cycle 1_{Cycle 5}ED,1 5 , D E x fI E slope 1 1 x fI E slope 5 5 (b)

Figure 7: Short cycle flexural response of the [(±45)5]slaminates for: (a)all 5 cycles and : (b)first and fifth

cycles. The energy dissipation for an n − th cycle ∆En is shown as well as the slopes for the first and fifth

cycles where the tested specimen flexural modulus of n − th cycle is Ef,n and the area moment of inertia

about the x-axis is Ix.

0 1 2 3 4 5 6 7 8 9 10 0 10 20 30 40 50 60 70 80 Number of Cycles, N E n e rg y d issi p a tio n f a co tr , d ( % ) [(75) 5]s [(60) 5]s [(45) 5]s [(30) 5]s [(0/90) 5]s

*Figure 8: Plots of energy dissipation for all the tested composites. Note: Solid trend lines indicate model*

*predictions while markers are experimental data.*

To quantify mathematically the dependence of percentage energy dissipation factor, ζd 262

with number of cycles, N , this study established that the numerical fit of the experimental 263

*data of Figure* *8* can be expressed by the power law:
264

ζd= ANb+ ζd,0 (6)

where ζd = energy dissipation factor, N = number of cycles, ζd,0 = threshold energy 265

dissipation factor and finally A, b are material constants. Typical values of A, b and ζd,0 for 266

*the laminates arrangements tested here are shown in Table* *3*.
267

*Equation* *3*represents a phenomenological model for characterizing the short cycle
flexu-268

ral response of PlytronTM *laminates. The A-parameter is a measure of first-cycle percentage*
269

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

Table 3: Typical values of material constants for the energy dissipation function associated with short cycle flexural behaviour of PlytronTM laminates.

Stacking Sequence A b ζd,0
[(0/90)5]s 5 -2.0 15
[(±30)5]_{s} 15 -2.0 26
[(±45)5]s 23 -2.0 35
[(±60)5]s 23 -2.0 36
[(±75)5]_{s} 30 -2.0 40

*change in energy dissipation. The A-parameter is high for laminate arrangements that show*
270

dominant plastic deformation (e.g. the [(±75)5]_{s} and [(±60)5]_{n} angle-ply laminates). The
271

ζd,0-parameter is a measure of the energy dissipation of the test material that remains con-272

stant with increasing number of cycles. Kar and co-workers [31] reported similar observation 273

for the bending fatigue of hybrid composites. 274

*5.4. Damage accumulation in cyclic flexural response*
275

With increasing number of cyclic loadings, the mechanical properties of composite ma-276

terials degrade progressively. The global damage caused by the cyclic flexural loading of 277

the test composite can be measured effectively by measuring the stiffness degradation of the 278

material [31–33]. An objective measure of this degradation is the global damage index, D 279

which can be defined as: 280 D = 1 −(EI)n (EI)1 , (7)

where (EI)n is the cyclic flexural rigidity after the n − th cycle, and (EI)1 is the flexural 281

rigidity after the first cycle for the tested cyclic deflection level, δlimit. These flexural moduli 282

are related to a chosen δlimit and should be differentiated from statically determined flexural 283

modulus, (EI)0 which is a reference value for monotonic flexural test deformed till failure 284

of the test material. Several microscopic damage mechanisms are assumed to contribute to 285

the D. For the thermoplastic matrix composites under investigation, these damage/failure 286

mechanisms are usually matrix-dominated and can include: matrix cracking (or more gen-287

erally inter-fibre failure), fibre-matrix debonding, ply delamination, fibre rupture and finally 288

fibre kinking[34]. Kar and co-workers [31] observed that with subsequent cycles, the micro-289

scopic damage continues to localize especially in the matrix and matrix-interphase phases 290

until eventual failure occurs. The final flexural rigidity at failure, (EI)f is calculated at the 291

last loading cycle before eventual failure. This will yield a GDI value of Df defined as global 292

damage index at failure of the test material. 293

*Combining Equation* *3* *and the cyclic flexural data of Figure* *5*, the flexural rigidity, EI
294

for each loading cycle was determined. These EI′_{s were then used with Equation}_{7}_{to}
295

*calculate the associated global damage index, D for the last n − th cycle (representative of*
296

*accumulated damage). The plot of the percentage global damage index, D against the tested*
297

*laminate arrangements is shown in Figure* *9*.
298

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

30 deg 45 deg 60 deg 75 deg 0/90 deg 0 20 40 60 80 100 Laminate Arrangements Glo ba l D am ag e Ind ex , D (%)

*Figure 9: Histogram of global damage index, D for all laminate arrangements. Note: D is expressed here*

*as a percentage, for easy interpretation of the extent of damage.*

*The result shown in Figure* *9* shows that damage accumulation was the most in the
299

[(±75)5]s laminates and the least in the [(±60)5]s laminates. The high damage accumula-300

tion seen in the [(±75)5]s indicates that for same cyclic deflection level (CDL), δlimit, more 301

microscopic damage occur than in say the [(±60)5]_{s} laminates. Gamstedt and Talreja [35]
302

investigated the fatigue damage mechanisms in unidirectional carbon-reinforced composites 303

with thermoset and thermoplastic matrices. The study showed the fatigue damage is a 304

cumulative effect of microscopic damage of the matrix and was particularly pronounced 305

in the thermoplastic (PEEK) matrix composites. These microscopic damages comprise of 306

widespread propagating debonds and matrix cracks. The authors did not assess the effect 307

of changing fibre orientation on the evolution of these microscopic damage. This evidence, 308

amongst several others, support the claim in this work that the observed damage accumula-309

*tion as shown in Figure9*is a consequence of progressively accumulating microscopic failure
310

mechanisms 311

6. Conclusions 312

The paper reports on the monotonic and cyclic flexural response of continuous E-glass 313

fibre reinforced polypropylene composites (marketed as PlytronTM ). By changing the ori-314

entation, θ of the fibre to the main bending axis, the flexural response of the laminates 315

changed from a linear elasticity dominant response until damage to a plasticity-dominant 316

response. Therefore, the effect of the matrix is significant in understanding the flexural 317

response of this type of thermoplastic matrix composite. Experimentally-derived flexural 318

modulus of all tested laminates were found to agree with predictions of the same based on 319

classical lamination theories. 320

Similarly, short cycle flexural response of PlytronTM was investigated for five stacking 321

sequences of the laminates. The study also developed a phenomenological model that de-322

scribes the dependence of energy dissipation with number of cycles. The study observed 323

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

that for all tested laminates, the largest energy dissipation occurred after the first cycle 324

and thereafter, the energy dissipation converges quickly to a cycle-independent energy dis-325

sipation value which is a material constant. This cycle-independent energy dissipation is 326

thought to be a saturated damaged state (or maximum energy-dissipation) within the test 327

material. The size of initial and saturated energy dissipation increases as the angle of fibre 328

orientation relative to the main bending axis increases too. 329

In conclusion, the flexural response of continuous E-glass fibre reinforced polypropylene 330

composites has been studied experimentally. It is concluded here that the plastic deforma-331

tion of the matrix contributes significantly to the flexural response. To encourage wider 332

application of this type of material in structural designs, it is imperative that a constitutive 333

model need to be developed. On evidence from this work, such model development must 334

consider the contribution of a robust matrix model towards the accurate prediction of the 335

mechanical response of PlytronTM . The experimental data presented here and the associ-336

ated phenomenological models will help in the micro-mechanical modelling for the class of 337

thermoplastic matrix composites as PlytronTM with a comparatively higher matrix volume 338

fraction. 339

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

References 340[1] Offringa, A.R.. Thermoplastic compositesrapid processing applications. Composites Part A: Applied

341

Science and Manufacturing 1996;27(4):329–336.

342

[2] Parlevliet, P.P., Bersee, H.E., Beukers, A.. Residual stresses in thermoplastic compositesa study of the

343

literaturepart i: Formation of residual stresses. Composites Part A: Applied Science and

Manufactur-344

ing 2006;37(11):1847 – 1857. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.compositesa.2005.12.025}.

345

URLhttp://www.sciencedirect.com/science/article/pii/S1359835X06000145.

346

[3] Stewart, R.. Thermoplastic compositesrecyclable and fast to process. Reinforced Plastics

347

2011;55(3):22–28.

348

[4] Sorrentino, L., Simeoli, G., Iannace, S., Russo, P.. Mechanical performance optimization through

in-349

terface strength gradation in pp/glass fibre reinforced composites. Composites Part B: Engineering

350

2015;76:201 – 208. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.compositesb.2015.02.026}. URL

351

http://www.sciencedirect.com/science/article/pii/S1359836815001122.

352

[5] Holbery, J., Houston, D.. Natural-fiber-reinforced polymer composites in automotive applications.

353

The Journal of The Minerals, Metals and Materials Society 2006;58(11):80–86. doi:\bibinfo{doi}{10.

354

1007/s11837-006-0234-2}. URLhttp://dx.doi.org/10.1007/s11837-006-0234-2.

355

[6] Ashori, A.. Woodplastic composites as promising green-composites for automotive industries!

356

Bioresource Technology 2008;99(11):4661 – 4667. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.

357

biortech.2007.09.043}. Exploring Horizons in Biotechnology: A Global Venture; URL http://www.

358

sciencedirect.com/science/article/pii/S0960852407007560.

359

[7] Fink, B.K.. Performance metrics for composite integral armor. Journal of Thermoplastic

Compo-360

site Materials 2000;13(5):417–431. doi:\bibinfo{doi}{10.1106/FR0L-T33W-JPD0-VFH3}. http:

361

//jtc.sagepub.com/content/13/5/417.full.pdf+html; URL http://jtc.sagepub.com/content/

362

13/5/417.abstract.

363

[8] Savage, G., Tacon, K., Welsh, I.. Composite armour materials. 1993. EP Patent 0,417,929; URL

364

https://www.google.com/patents/EP0417929B1?cl=en.

365

[9] Villanueva, G.R., Cantwell, W.. The high velocity impact response of composite and fml-reinforced

366

sandwich structures. Composites Science and Technology 2004;64(1):35 – 54. doi:\bibinfo{doi}{http:

367

//dx.doi.org/10.1016/S0266-3538(03)00197-0}. URL http://www.sciencedirect.com/science/

368

article/pii/S0266353803001970.

369

[10] Abdullah, M., Cantwell, W.. The impact resistance of polypropylene-based fibremetal laminates.

370

Composites Science and Technology 2006;66(1112):1682 – 1693. doi:\bibinfo{doi}{http://dx.doi.org/

371

10.1016/j.compscitech.2005.11.008}. URL http://www.sciencedirect.com/science/article/pii/

372

S0266353805004203.

373

[11] Carrillo, J., Cantwell, W.. Mechanical properties of a novel fibermetal laminate based on a

poly-374

propylene composite. Mechanics of Materials 2009;41(7):828 – 838. doi:\bibinfo{doi}{http://dx.doi.

375

org/10.1016/j.mechmat.2009.03.002}. URLhttp://www.sciencedirect.com/science/article/pii/

376

S0167663609000593.

377

[12] Jen, M.H., Lee, C.H.. Strength and life in thermoplastic composite laminates under

378

static and fatigue loads. part i: Experimental. International Journal of Fatigue 1998;20(9):605

379

– 615. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/S0142-1123(98)00029-2}. URL http://www.

380

sciencedirect.com/science/article/pii/S0142112398000292.

381

[13] Hwang, J.S., Choi, T.G., Lee, D., Lyu, M.Y., Lee, D.G., Yang, D.Y.. Dynamic and static

382

characteristics of polypropylene pyramidal kagome structures. Composite Structures 2015;131:17

383

– 24. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.compstruct.2015.04.065}. URL http://www.

384

sciencedirect.com/science/article/pii/S0263822315003608.

385

[14] Eksi, S., Genel, K.. Bending response of hybrid composite tubular beams. Thin-Walled Structures

386

2013;73:329 – 336. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.tws.2013.09.001}. URLhttp://www.

387

sciencedirect.com/science/article/pii/S0263823113002164.

388

[15] GuritSuprem, . Material safety data sheet - plytron: According to ec directive 91/155/eec. Tech. Rep.;

389

GuritSuprem; 2004.

390

[16] GuritSuprem, . Plytron - product description, properties and applications - a technical report. Tech.

391

Rep.; Gurit Composite Technologies; 2005.

392

[17] Al-Zubaidy, M., Chan, J., Gibson, A., Toll, S.. Properties of orthotropic glasspolypropylene

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

composites manufactured by weaving of prepregtapes and other routes. Plastics, Rubber and

Compo-394

sites 2000;29(10):520–526. doi:\bibinfo{doi}{10.1179/146580100101540725}.http://dx.doi.org/10.

395

1179/146580100101540725; URLhttp://dx.doi.org/10.1179/146580100101540725.

396

[18] Santulli, C., Brooks, R., Long, A.C., Warrior, N.A., Rudd, C.D.. Impact properties of

com-397

pression moulded commingled e-glasspolypropylene composites. Plastics, Rubber and Composites

398

2002;31(6):270–277. doi:\bibinfo{doi}{10.1179/146580102225004983}. http://dx.doi.org/10.1179/

399

146580102225004983; URLhttp://dx.doi.org/10.1179/146580102225004983.

400

[19] Rijsdijk, H., Contant, M., Peijs, A.. Special issue microphenomena in advanced composites

401

continuous-glass-fibre-reinforced polypropylene composites: I. influence of maleic-anhydride-modified

402

polypropylene on mechanical properties. Composites Science and Technology 1993;48(1):161 – 172. doi:

403

\bibinfo{doi}{http://dx.doi.org/10.1016/0266-3538(93)90132-Z}. URLhttp://www.sciencedirect.

404

com/science/article/pii/026635389390132Z.

405

[20] Thomason, J., Schoolenberg, G.. An investigation of glass fibre/polypropylene interface strength and

406

its effect on composite properties. Composites 1994;25(3):197 – 203. doi:\bibinfo{doi}{http://dx.doi.

407

org/10.1016/0010-4361(94)90017-5}. URLhttp://www.sciencedirect.com/science/article/pii/

408

0010436194900175.

409

[21] Yang, L., Thomason, J.. Interface strength in glass fibrepolypropylene measured using the fibre

pull-410

out and microbond methods. Composites Part A: Applied Science and Manufacturing 2010;41(9):1077

411

– 1083. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.compositesa.2009.10.005}. Special Issue on 10th

412

Deformation and Fracture of Composites Conference: Interfacial interactions in composites and other

413

applications; URLhttp://www.sciencedirect.com/science/article/pii/S1359835X09003157.

414

[22] Hagstrand, P.O., Bonjour, F., Mnson, J.A.. The influence of void content on the structural

flex-415

ural performance of unidirectional glass fibre reinforced polypropylene composites. Composites Part

416

A: Applied Science and Manufacturing 2005;36(5):705 – 714. doi:\bibinfo{doi}{http://dx.doi.org/

417

10.1016/j.compositesa.2004.03.007}. URL http://www.sciencedirect.com/science/article/pii/

418

S1359835X04000740.

419

[23] Simeoli, G., Acierno, D., Meola, C., Sorrentino, L., Iannace, S., Russo, P.. The role of

inter-420

face strength on the low velocity impact behaviour of pp/glass fibre laminates. Composites Part B:

421

Engineering 2014;62:88 – 96. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.compositesb.2014.02.018}.

422

URLhttp://www.sciencedirect.com/science/article/pii/S135983681400095X.

423

[24] Russo, P., Acierno, D., Simeoli, G., Iannace, S., Sorrentino, L.. Flexural and impact response

424

of woven glass fiber fabric/polypropylene composites. Composites Part B: Engineering 2013;54:415

425

– 421. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.compositesb.2013.06.016}. URL http://www.

426

sciencedirect.com/science/article/pii/S1359836813003272.

427

[25] Gibson, R.. Principles of Composite Material Mechanics, Third Edition. Mechanical Engineering;

428

Taylor & Francis; 2011. ISBN 9781439850053. URL https://books.google.co.uk/books?id=

429

vxg9Z4aJ36MC.

430

[26] Jones, R.. Mechanics Of Composite Materials. Materials Science and Engineering Series; Taylor &

431

Francis; 1998. ISBN 9781560327127. URLhttps://books.google.co.uk/books?id=oMph2kNG3yAC.

432

[27] Chamis, C.C.. Simplified composite micromechanics for predicting microstresses. Journal of Reinforced

433

Plastics and Composites 1987;6(3):268–289. doi:\bibinfo{doi}{10.1177/073168448700600305}. http:

434

//jrp.sagepub.com/content/6/3/268.full.pdf+html; URL http://jrp.sagepub.com/content/

435

6/3/268.abstract.

436

[28] de Morais, A.B.. Transverse moduli of continuous-fibre-reinforced polymers. Composites Science

437

and Technology 2000;60(7):997 – 1002. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/S0266-3538(99)

438

00195-5}. URLhttp://www.sciencedirect.com/science/article/pii/S0266353899001955.

439

[29] Paepegem, W.V., Geyter, K.D., Vanhooymissen, P., Degrieck, J.. Effect of friction on the

hystere-440

sis loops from three-point bending fatigue tests of fibre-reinforced composites. Composite Structures

441

2006;72(2):212 – 217. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.compstruct.2004.11.006}. URL

442

http://www.sciencedirect.com/science/article/pii/S0263822304003794.

443

[30] Sakin, R., rfan Ay, , Yaman, R.. An investigation of bending fatigue behavior for

glass-444

fiber reinforced polyester composite materials. Materials & Design 2008;29(1):212 – 217. doi:

445

\bibinfo{doi}{http://dx.doi.org/10.1016/j.matdes.2006.11.006}. URL http://www.sciencedirect.

446

com/science/article/pii/S0261306906003451.

## M

## A

## N

## U

## S

## C

## R

## IP

## T

## A

## C

## C

## E

## P

## T

## E

## D

[31] Kar, N., Barjasteh, E., Hu, Y., Nutt, S.. Bending fatigue of hybrid composite rods. Composites

448

Part A: Applied Science and Manufacturing 2011;42(3):328 – 336. doi:\bibinfo{doi}{http://dx.doi.org/

449

10.1016/j.compositesa.2010.12.012}. URL http://www.sciencedirect.com/science/article/pii/

450

S1359835X10003283.

451

[32] Mao, H., Mahadevan, S.. Fatigue damage modelling of composite materials. Composite Structures

452

2002;58(4):405 – 410. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/S0263-8223(02)00126-5}. URL

453

http://www.sciencedirect.com/science/article/pii/S0263822302001265.

454

[33] Wu, F., Yao, W.. A fatigue damage model of composite materials. International Journal of Fatigue

455

2010;32(1):134 – 138. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/j.ijfatigue.2009.02.027}. Fourth

In-456

ternational Conference on Fatigue of Composites (ICFC4); URL http://www.sciencedirect.com/

457

science/article/pii/S0142112309000747.

458

[34] Brinson, H.F.. Matrix dominated time dependent failure predictions in polymer matrix

compo-459

sites. Composite Structures 1999;47(14):445 – 456. doi:\bibinfo{doi}{http://dx.doi.org/10.1016/

460

S0263-8223(00)00075-1}. Tenth International Conference on Composite Structures; URL http:

461

//www.sciencedirect.com/science/article/pii/S0263822300000751.

462

[35] Gamstedt, E., Talreja, R.. Fatigue damage mechanisms in unidirectional

carbon-fibre-463

reinforced plastics. Journal of Materials Science 1999;34(11):2535–2546. doi:\bibinfo{doi}{10.1023/A:

464

1004684228765}. URLhttp://dx.doi.org/10.1023/A%3A1004684228765.